N A N O E X P R E S S
Large-Area Growth of Uniform Single-Layer
Thin Films by Chemical Vapor Deposition
Seung Hyun Baek, Yura Choi and Woong Choi*
We report the largest-size thin films of uniform single-layer MoS2on sapphire substrates grown by chemical vapor deposition based on the reaction of gaseous MoO3and S evaporated from solid sources. The as-grown thin films of single-layer MoS2were continuous and uniform in thickness for more than 4 cm without the existence of
triangular-shaped MoS2clusters. Compared to mechanically exfoliated crystals, the as-grown single-layer MoS2thin films possessed consistent chemical valence states and crystal structure along with strong photoluminescence emission and optical absorbance at high energy. These results demonstrate that it is possible to scale up the growth of uniform single-layer MoS2thin films, providing potentially important implications on realizing high-performance MoS2devices.
Keywords:MoS2; Single layer; Thin films; Chemical vapor deposition PACS:81.05.Hd; 81.10.Bk; 81.15.Gh
Two-dimensional transition metal dichalcogenides (TMDs) have received great attention because of their interesting electronic, optical, and chemical properties. Among various TMDs, molybdenum disulfide (MoS2) has been most extensively investigated for the applications of thin-film transistors (TFTs), photodetectors, and energy storage [1–3]. TFTs based on single- or multilayer MoS2exhibit intriguing transistor performance including high on/off current ratio (~107), high mobility at room temperature (~100 cm2 V−1 s−1), and low subthreshold swing (~70 mV decade−1) [4, 5]. Moreover, photodetectors based on single- or multilayer MoS2show high photo-responsivity (300–800 A W−1) exceeding that of silicon-based ones [6, 7]. However, the aforementioned examples have been demonstrated using mechanically exfoliated MoS2flakes, which are typically micrometer-scale in size. Hence, the growth of large-area MoS2 is one of the critical challenges to realize its promising potential.
So far, a variety of synthesis approaches have been re-ported to grow large-area MoS2 including liquid exfoli-ation (sonicexfoli-ation in solvents) , two-step chemical vapor deposition (CVD, sulfurization or decomposition of pre-deposited Mo-based thin films) [9–11], one-step CVD (reaction of gaseous Mo and S precursors) [12–14], and physical vapor deposition (sputtering and pulsed laser deposition) [15, 16]. Special emphasis has been put on one-step CVD as it shows greater potential for growing uniform large-grain thin films of single-layer MoS2. The most common one-step CVD is based on the reaction of gaseous MoO3and S evaporated from solid sources due to the simplicity of processing and the easy avail-ability of solid sources . When the optimized CVD process conditions with MoO3 and S precursors are combined with the use of mica or substrate treatment, the formation of single-layer MoS2 thin films can be obtained up to about a centimeter [17–19]. However, CVD processes based on MoO3 and S powders typic-ally result in triangular-shaped discontinuous clusters of either single-layer MoS2or mixtures of single- and few-layer MoS2 . Therefore, more work is needed to establish a CVD process that can reproducibly pro-vide continuous large-area thin films of uniform single-layer MoS2.
School of Advanced Materials Engineering, Kookmin University, Seoul 02707, South Korea
Here, we investigate CVD methods based on MoO3and S powders to grow continuous thin films of single-layer MoS2 for more than 4 cm on sapphire substrates. Our MoS2 thin films are the largest in size grown by CVD methods based on MoO3and S powders. The large-area deposition, thickness uniformity, and crystallinity of single-layer MoS2thin films are confirmed by scanning electron microscopy (SEM), atomic force microscopy (AFM), x-ray photoelectron spectroscopy (XPS), Raman spectroscopy, photoluminescence (PL) spectroscopy, ultraviolet (UV)-vis-ible spectroscopy, and transmission electron microscopy (TEM).
MoS2films were deposited on (0001)-oriented sapphire substrates in a two-zone tube furnace. MoO3 (99.98 %, Sigma-Aldrich) and S (99.98 %, Sigma-Aldrich) powders
in two separate Al2O3 boats were used as precursors. MoO3 powder (15 mg) was placed upstream at zone 1 (700 °C), and S powder (1 g) was placed at the upstream entry of the furnace. The substrates were placed down-stream at zone 2 (600 °C). MoO3powder was heated up to 700 °C at a rate of 15 °C min−1, and the substrates were heated up to 600 °C at 38 °C min−1. After 30-min deposition, the furnace was slowly cooled down to room temperature. Ar flow of 100 sccm and a pressure of ~0.5 Torr were maintained during deposition.
The surface morphology of deposited thin films was observed by SEM (JEOL JSM-7610F) and AFM (Park Systems XE-100). Elemental composition was analyzed using XPS (PHI X-tool). The thickness and uniformity of deposited thin films were measured by Raman and PL spectra (Horiba LabRAM Aramis) using a laser of 532 nm in wavelength. Optical
absorbance was measured by UV-visible spectroscopy (PerkinElmer Lambda 35). Crystal structure was ana-lyzed by TEM (FEI Titan 80–300) at 300 kV.
Results and Discussion
MoS2 thin films deposited on sapphire substrates are light yellow-green in color exhibiting obvious color con-trast with transparent bare sapphire substrates as shown in Fig. 1a. The continuous formation of MoS2thin films is observed up to 4 cm. The existence of MoS2thin films on substrates can be confirmed by the color contrast in the SEM image of an intentionally scratched sample in Fig. 1b. When MoO3and S powders are used as precur-sors, triangular-shaped discontinuous clusters of either single-layer MoS2 or mixtures of single- and few-layer MoS2are typically observed in literature . Similarly, triangular-shaped clusters or regions of bilayer MoS2 can be observed in this investigation when process con-ditions are not optimized (see Additional file 1). How-ever, with optimized process conditions, such triangular clusters of MoS2cannot be found in our MoS2thin films as shown Fig. 1b. The absence of triangular clusters of MoS2 is further confirmed by AFM image in Fig. 1c. The AFM measurement on the scratched sample in Fig. 1d shows thickness of 0.7 nm corresponding to that of single-layer MoS2. As MoS2 growth is known to be sensitive to the localized concentration of precursors , the combination of the low pressure, distance be-tween precursors and substrates, and temperature used in this investigation may result in uniform nucleation and growth of MoS2. Figure 1e, f compares XPS of the deposited MoS2thin films with that of bulk MoS2single crystals. The existence of Mo4+ (Mo 3d5/2 orbital at 229.1 eV and Mo 3d3/2orbital at 232.3 eV) and S2−(S 2p3/2 orbital at 162.0 eV and S 2p1/2orbital at 163.1 eV) is clearly seen in our thin films.
To confirm the thickness of deposited MoS2thin films, we measure the Raman spectra of deposited MoS2 thin films. Figure 2a shows the two characteristic Raman A1g and E12g modes of four different MoS2 samples—CVD MoS2thin films on sapphire substrates, CVD MoS2 thin films transferred on SiO2/Si substrates, mechanically exfo-liated single-layer MoS2flakes on SiO2/Si substrates, and bulk MoS2 single crystals. The frequency difference be-tween A1g and E12g modes (Δ) of MoS2 is related to its thickness . Except bulk single crystals (Δ= 25.1 cm−1), all other MoS2 samples possess Δ between 19.6 and 19.9 cm−1 suggesting single-layer MoS2. It needs to be mentioned that the positions of A1g and E12g modes are slightly shifted for single-layer MoS2on SiO2/Si substrates (both transferred CVD films and mechanically exfoliated MoS2flakes). This is due to the effect of underlying SiO2/ Si substrates as substrates can strongly affect the Raman and PL emission of single-layer MoS2.
The thickness of MoS2thin films is further confirmed by PL spectra. While the indirect bandgap of multilayer MoS2does not allow PL emission, the direct bandgap of
single-layer MoS2allows PL emission [23, 24]. Figure 2b
shows the PL spectra of the same four MoS2
sam-ples—CVD MoS2 thin films on sapphire substrates, CVD MoS2thin films transferred on SiO2/Si substrates, mechanically exfoliated single-layer MoS2 flakes on SiO2/Si substrates, and bulk MoS2single crystals. While the emission intensity completely disappears for bulk MoS2, our single-layer MoS2thin films on sapphire show a PL emission peak at 1.88 eV confirming they are single-layer MoS2. The PL spectrum of our single-layer MoS2 thin films on sapphire is different from that of mechanically exfoliated single-layer MoS2 flakes on SiO2/Si. Two emission peaks are observed for mechanic-ally exfoliated single-layer MoS2 flakes on SiO2/Si at 1.85 and 2.00 eV known as A and B direct excitonic transitions [23, 24]. The shift of emission peak A and the absence of emission peak B in our single-layer MoS2 thin films on sapphire are due to the effect of the under-lying substrate . The consistent PL emission spectrum from transferred single-layer MoS2 on SiO2/Si with that of mechanically exfoliated single-layer MoS2flakes on SiO2/Si supports this.
The UV-visible absorption spectrum in Fig. 2c shows A and B absorption due to excitonic transitions along with C and D absorption associated with van Hove singularity [25, 26]. As the existence of van Hove
singularity can enhance light-matter interactions, single-layer MoS2 thin films may be suitable for photovoltaic cells and photodetectors due to enhanced photon absorp-tion and electron-hole creaabsorp-tion.
We also perform TEM analysis to obtain information on the crystallinity of the single-layer MoS2 thin films. The low-magnification bright-field TEM cross-sectional image in Fig. 3a shows continuous single-layer MoS2 thin films on sapphire substrates. The high-resolution plan-view image in Fig. 3b and the corresponding fast Fourier transformation pattern in its inset reveal the hexagonal crystal structure of single-layer MoS2 thin films. The estimated interplanar spacing of (100) and (110) planes is ~0.28 and ~0.16 nm, respectively, which is in good agreement with literature . The selected area electron diffraction (SAED) pattern obtained from the low-magnification plan-view image in Fig. 3c shows multiple rings confirming the polycrystalline nature of the MoS2thin films.
For more quantitative assessment of the thickness uni-formity, Raman and PL spectra are measured at eight different positions of a 4-cm-wide single-layer MoS2thin film (insets of Fig. 4a, b). Figure 4a, b shows negligible variation of the measured full-width at half maximum (FWHM) of Raman A1gand E12gmodes,Δ, FWHM of PL emission peak, and PL emission wavelength. Figure 4c, d
shows the measured Raman A1gmode frequency and PL emission wavelength based on mapping over an area of 10μm × 10μm, respectively. Measured Raman A1gmode frequency and PL emission wavelength exist in a range of 406.1–406.3 cm−1 and 659–662 nm, respectively. These results suggest that the thickness of our single-layer MoS2 thin films is uniform across the substrate.
In summary, we synthesized uniform large-area thin films of single-layer MoS2 on sapphire substrates by CVD based on MoO3 and S precursors. The as-grown thin films were composed of single-layer MoS2and con-tinuous for more than 4 cm without triangular-shaped clusters of MoS2. The chemical configuration, thickness, thickness uniformity, and crystalline quality of MoS2 thin films were confirmed by XPS, AFM, Raman and PL spectra, and TEM analysis. The optical absorbance meas-urement further suggested the existence of van Hove sin-gularity at high energy. These results will help scale up the growth of two-dimensional TMDs, providing potentially important implications on realizing the promising poten-tial of high-performance MoS2devices such as thin-film transistors, sensors, and photodetectors.
Additional file 1:Formation of nonuniform MoS2clusters.
(DOCX 379 kb)
The authors declare that they have no competing interests.
SB and WC initiated the research and analyzed experimental data. SB worked on the growth and characterization of CVD thin films. YC worked on the fabrication and characterization of mechanically exfoliated single-layer flakes. WC wrote the manuscript. All authors read and approved the final manuscript.
This work was supported by the National Research Foundation of Korea (Grant 2013R1A1A2008191, 2013K1A4A3055679, and NRF-2013K1A3A1A32035549) and Industrial Strategic Technology Development Program (Grant 10045145).
Received: 17 August 2015 Accepted: 27 September 2015
1. Lembke D, Bertolazzi S, Kis A (2015) Single-layer MoS2electronics. Acc Chem Res 48:100–110
2. Xia F, Wang H, Xiao D, Dubey M, Ramasubramaniam A (2014) Two-dimensional material nanophotonics. Nat Photon 8:899–907 Fig. 4aFWHM of Raman E1
2gand A1gmodes along withΔ(red diamond:Δ, white square: FWHM of Raman A1gmode, blue square: FWHM of Raman E1
3. Bonaccorso F, Colombo L, Yu G, Stoller M, Tozzini V, Ferrari AC, Ruoff RS, Pellegrini V (2015) Graphene, related two-dimensional crystals, and hybrid systems for energy conversion and storage. Science 347:1246501 4. Radisavljevic B, Radenovic A, Brivio J, Giacometti V, Kis A (2011) Single-layer
MoS2transistors. Nat Nanotechnol 6:147–50
5. Kim S, Konar A, Hwang WS, Lee JH, Lee J, Yang J, Jung C, Kim H, Yoo JB, Choi JY, Jin YW, Lee SY, Jena D, Choi W, Kim K (2012) High-mobility and low-power thin-film transistors based on multilayer MoS2crystals. Nat Commun 3:1011 6. Lopez-Sanchez O, Lembke D, Kayci M, Radenovic A, Kis A (2013) Ultrasensitive
photodetectors based on monolayer MoS2. Nat Nanotech 8:497–501 7. Kwon J, Hong YK, Han G, Omkaram I, Choi W, Kim S, Yoon Y (2015) Giant
photoamplification in indirect-bandgap multilayer MoS2phototransistors with local bottom-gate structures. Adv Mater 27:2224–30
8. Coleman JN, Lotya M, O’Neill A, Bergin SD, King PJ, Khan U, Young K, Gaucher A, De S, Smith RJ, Shvets IV, Arora SK, Stanton G, Kim H-Y, Lee K, Kim GT, Duesberg GS, Hallam T, Boland JJ, Wang JJ, Donegan JF, Grunlan JC, Moriarty G, Shmeliov A, Nicholls RJ, Perkins JM, Grieveson EM, Theuwissen K, McComb DW, Nellist PD, Nicolosi V (2011) Two-dimensional nanosheets produced by liquid exfoliation of layered materials. Science 331:568–71 9. Liu KK, Zhang W, Lee Y-H, Lin Y-C, Chang M-T, Su C-Y, Chang C-S, Li H, Shi
Y, Zhang H, Lai C-S, Li L-J (2012) Growth of large-area and highly crystalline MoS2thin layers on insulating substrates. Nano Lett 12:1538–44
10. Zhan Y, Liu Z, Najmaei S, Ajayan PM, Lou J (2012) Large-area vapor-phase growth and characterization of MoS2atomic layers on a SiO2Substrate. Small 8:966–71
11. Lin Y-C, Zhang W, Huang J-K, Liu K-K, Lee Y-H, Liang C-T, Chu C-W, Li L-J (2012) Wafer-scale MoS2thin layers prepared by MoO3sulfurization. Nanoscale 4:6637–41
12. Lee Y-H, Zhang X-Q, Zhang W, Chang M-T, Lin C-T, Chang K-D, Yu Y-C, Wang JT-W, Chang C-S, Li L-J, Lin T-W (2012) Synthesis of large-area MoS2 atomic layers with chemical vapor deposition. Adv Mater 24:2320–25 13. Yu Y, Li C, Liu Y, Su L, Zhang Y, Cao L (2013) Controlled scalable synthesis of
uniform, high-quality monolayer and few-layer MoS2films. Sci Rep 3:1866 14. Kang K, Xie S, Huang L, Han Y, Huang PY, Mak KF, Kim C-J, Muller D, Park J
(2015) High-mobility three-atom-thick semiconducting films with wafer-scale homogeneity. Nature 520:656–60
15. Serrao CR, Diamond AM, Hsu S-L, You L, Gadgil S, Clarkson J, Carraro C, Maboudian R, Hu C, Salahuddin S (2015) Highly crystalline MoS2thin films grown by pulsed laser deposition. Appl Phys Lett 106:052101
16. Ling ZP, Yang R, Chai JW, Wang SJ, Leong WS, Tong Y, Lei D, Zhou Q, Gong X, Chi DZ, Ang K-W (2015) Large-scale two-dimensional MoS2
photodetectors by magnetron sputtering. Opt Exp 23:13580–86
17. Ji Q, Zhang Y, Gao T, Zhang Y, Ma D, Liu M, Chen Y, Qiao X, Tan P-H, Kan M, Feng J, Sun Q, Liu Z (2013) Epitaxial monolayer MoS2on mica with novel photoluminescence. Nano Lett 13:3870–77
18. Dumcenco D, Ovchinnikov D, Marinov K, Lazic P, Gibertini M, Marzari N, Lopez-Sanchez O, Kung Y-C, Krasnozhon D, Chen M-W, Bertolazzi S, Gillet P, Fontcuberta i Morral A, Radenovic A, Kis A (2015) Large-area epitaxial monolayer MoS2. ACS Nano 9:4611–20
19. Jeon J, Jang SK, Jeon SM, Yoo G, Jang YH, Park J-H, Lee S (2015) Layer-controlled CVD growth of large-area two-dimensional MoS2films. Nanoscale 7:1688–95 20. Ji Q, Zhang Y, Zhang Y, Liu Z (2015) Chemical vapour deposition of
group-VIB metal dichalcogenide monolayers: engineered substrates from amorphous to single crystalline. Chem Soc Rev 44:2587–602 21. Lee C, Yan H, Brus LE, Heinz TF, Hone J, Ryu S (2010) Anomalous lattice
vibrations of single and few-layer MoS2. ACS Nano 4:2695–700
22. Buscema M, Steele GA, van der Zant HSJ, Castellanos-Gomez A (2014) The effect of the substrate on the Raman and photoluminescence emission of single-layer MoS2. Nano Res 7:561–71
23. Splendiani A, Sun L, Zhang Y, Li T, Kim J, Chim C, Galli G, Wang F (2010) Emerging photoluminescence in monolayer MoS2. Nano Lett 10:1271–5 24. Mak KF, Lee C, Hone J, Shan J, Heinz TF (2010) Atomically thin MoS2: a new
direct-gap semiconductor. Phys Rev Lett 105:136805
25. Britnell L, Ribeiro RM, Eckmann A, Jalil R, Belle BD, Mishchenko A, Kim Y-J, Gorbachev RV, Georgiou T, Morozov SV, Grigorenko AN, Geim AK, Casiraghi C, Castro Neto AH, Novoselov KS (2013) Strong light-matter interactions in heterostructures of atomically thin films. Science 340:1311–4
26. Klots AR, Newaz AKM, Wang B, Prasai D, Krzyzanowska H, Lin J, Caudel D, Ghimire NJ, Yan J, Ivanov BL, Velizhanin KA, Burger A, Mandrus DG, Tolk NH, Pantelides ST, Bolotin KI (2014) Probing excitonic states in suspended two-dimensional semiconductors by photocurrent spectroscopy. Sci Rep 4:6608
Submit your manuscript to a
journal and beneﬁ t from:
7Convenient online submission
7Rigorous peer review
7Immediate publication on acceptance
7Open access: articles freely available online
7High visibility within the ﬁ eld
7Retaining the copyright to your article